Comparative Evaluation of Flexural Strength of Provisional Crown and Bridge Materials-An Invitro Study
Ankita Singh1, Sandeep Garg2
ABSTRACT Introduction: Provisional restorations serve a key role as a functional and esthetic try-in for the design of the final prosthesis. During selection of materials for this restoration, clinicians must consider physical properties, ease of handling, cost and patient satisfaction and approval. Aim: To evaluate and compare the flexural strength of provisional crown and bridge materials available commercially. Materials and Methods: This in-vitro study was done to compare the flexural strength of six temporary crown and bridge materials available commercially at 24 hours, 8 days and after repair. Three poly methyl methacrylate based materials (DPI, SC10 and Trulon) and three bis-acrylic based composite resins (Protemp, Cooltemp and Luxatemp) were selected. A total of 72 specimens of dimensions 64mm×10mm×2.5mm were prepared from these materials (12 from each material) and divided into two groups (n=36). Specimens were stored in artificial saliva and were fractured after 24 hours and 8 days using Universal Testing Machine. The fractured samples from the 8 days study
were then subjected to repair. A uniform space of 2mm and a 450 bevel was maintained for all the repaired samples for better distribution of forces. Flexural strength of these repaired samples was recorded using the same machine. Results were recorded and statistically analysed by one-way Anova and Post hoc tests. Result: Results revealed that there was decrease in flexural strength for all the materials tested from 24 hours to 8 days, though flexural strength between poly methyl methacrylate and bis-acrylic resins was similar at 24 hours and 8 days time interval. A substantial decrease was noticed in the strength of bis-acrylic composite resins after repair. Conclusion: From the current study it can be suggested that though there is decrease in flexural strength for all the materials from 24 hours to 8 days, both can be used to fabricate the provisional restorations. However, in the event of a fracture of a bis-acrylic provisional restoration, it may be more advantageous to make a new provisional restoration than to repair the fractured one.
Keywords: Acrylic resins, Bis-acryl composite resins, Interim dental prosthesis, Poly methyl methacrylate, Temporization
Introduction Fixed prosthodontic treatment involves complete or partial coverage of natural tooth or dental implant abutments. It depends on fabrication of a definitive prosthesis in the dental laboratory . Fabrication of the final prosthesis takes about 8-10 days. During this time period, the prepared tooth needs to be protected from the oral environment and its relationship with the adjacent and opposing tooth needs to be preserved. Hence, in order to protect these prepared abutment teeth, temporary restorations are fabricated. These interim restorations are also beneficial for diagnostic purposes where the functional, stabilizing, occlusal and esthetic parameters are developed to identify an optimum treatment result before the completion of definitive prosthesis . While selecting a material for a temporary restoration, physical and mechanical properties of the materials should be considered. Clinically significant properties include strength of the material, its rigidity and reparability, exothermic reaction following polymeri zation and subsequent polymerization shrinkage, marginal integrity and colour stability . Presently there is no single material that meets the optimal requirements for all the situations . However, there are materials that have been successfully used for this purpose. These are Poly Methyl Methacrylate Resins (PMMA), Poly Ethyl Methacrylate Resins (PEMA), vinyl ethyl methacrylate resins, butyl methacrylate, epimine, preformed matrices of plastic and cellulose shells, metals, polycarbonate materials, bis-acryl composites, bis-GMA composites, Urethane Di Methacrylate Resins (UDMA) . 72
The most common materials for custom interim fixed partial denture are acrylic resins. PMMA were introduced in 1936 as a heat processed thermosetting material. In early 1940’s, it was available as a room temperature polymerizing methacrylate. It was quickly improved for the field of dentistry as a self-curing prosthetic and restorative resin . Acrylic based resins consist of polymeric materials based on PMMA. These materials are a result of a free radical polymerization reaction initiated chemically. PMMA resins are relatively inexpensive with ease of handling, excellent polish and good marginal adaptation. The major drawback of these materials is the exothermic polymerization; high polymerization shrinkage and low wear resistance . Bis-acryl composite were introduced with an aim to overcome the negatives of the methacrylate . They are available as preloaded syringes or cartridges and mixed through an auto mixing tip. This provides consistent mixture with no air incorporation into the final mix . Bis-acryl composites consist of bi-functional substrates to provide cross linkage with one another and form monomer chain cross linkage leading to increase in impact strength and toughness . They also contain inorganic fillers to increase their abrasion resistance. Bis-acryl composite resins have low polymerization shrinkage , low exothermic reaction, reduced tissue toxicity, good wear resistance and strength. But these materials are expensive, brittle and have less polish ability and their repair is difficult . Wang RL et al., in 1989 and Osman YI et al., in 1993 found that methyl methacrylate provisional materials had higher flexural strength than the composite material [9,10]. Journal of Clinical and Diagnostic Research. 2016 Aug, Vol-10(8): ZC72-ZC77
Ankita Singh and Sandeep Garg, Comparative Evaluation of Flexural Strength of Provisional Crown and Bridge Materials- An In-vitro Study
On the contrary Young HM et al., compared bis-acryl and PMMA materials in terms of occlusion, contour, marginal adaptability and finish . For both anterior and posterior teeth, they found the bis acryl material significantly superior to PMMA in all categories. Due to this confusion and the urge to determine and predict the possible reasons for such discrepancy, an attempt was made to evaluate and compare the flexural strength of these two main groups of temporary crown and bridge materials.
MATERIALS AND METHODS This in-vitro study was conducted in the Department of Prosthodontics including Crown and Bridge, M. M. College of Dental Sciences and Research, Mullana, (Ambala), Haryana, India and Central Institute of Plastics Engineering and Technology, Murthal (Sonipat), Haryana, India. The study period was almost a month. Six commercially available temporary fixed partial denture materials considered were: 1. Poly methyl methacrylate based temporary materials available in powder liquid form: a. DPI self-cure tooth molding powder (DPI, The Bombay Burmah Trading Corp. Ltd., Batch 3152, Mumbai, India). b. SC10 tooth colored cold cure (Jagdish Lal Sethi Company, Batch SC411, Wazirpur, Delhi, India).
specimens from each material) and were stored in artificial saliva in labelled plastic jars. Specimens were tested at a time interval of 24 hours and 8 days respectively using Instron Universal Testing Machine having a maximum capacity of 100 KN and a digital recording system [Table/Fig-3]. Three point bending test was performed at a crosshead speed of 5mm/minute until failure and flexural strength was recorded for all specimens. The force was calculated in Newton (N) and converted to stress (N/mm2). The broken specimens from the 8 day study were collected, washed and cleaned. The numbering done previously on the corresponding ends allowed realignment in the original position [Table/Fig-4]. An equal gap between the fractured ends of all samples was planned to maintain the standardizations and to provide space for the material to flow. A distance of 1mm from each side of the fractured line was marked. The sample was cut at these lines with a separating disk and the ends were finished. For all the samples, the space between the edges to be repaired when placed in the mould was 2mm. Also a 450 degree bevel was prepared to increase the inter-facial bond area. To achieve that, a distance equal to the thickness of the sample (2.5mm) from the prepared edge was measured and a line parallel to the edge was drawn at this point. The upper end of this line and the lower end of the edge to be repaired were joined. The trimming along the line
c. Trulon acrylic crown and bridge Trulon (Jayna Industries, Ghaziabad, UP, India). 2. Bis-acryl composite based temporary materials available as cartridge with dispensing gun and mixing tips: a. Protemp 4 temporization material (3M ESPE, Lot 559121, Germany). b. Cooltemp natural (Coltene Whaledent, Lot F27307, Article no5805, Switzerland). c.
Luxatemp fluorescence Germany).
A custom made metal mould was used for making specimens. It was a rectangular mold with five slots of dimensions 64mm×10mm×2.5mm [Table/Fig-1]. It was open on one side with adjustable screws on the ends to carefully remove the samples. Twelve specimens for each material were prepared in the form of rectangular bars. Petroleum jelly was applied on inner surface of the mould with the help of a brush. PMMA resins were manipulated according to manufacturer’s instructions in a dappen dish using a mixing spatula. The mix was expressed into the mould slots to its capacity and a glass slab was pressed tightly against the mould to remove excess material. For the bis-acryl composites, the material was dispensed into the slots directly using a dispensing gun. The material was allowed to set. Once material was set, the adjustment screws were loosened. Specimens were removed from the mould, excess was trimmed and finishing was done. A total of 72 samples were prepared and marked with a specific number describing the type of material and the order of their fabrication [Table/Fig-2]. The marking was done on both ends to facilitate the relocation of broken samples during repair procedures. All specimens were divided into two groups consisting of 36 specimens each (six
[Table/Fig-4]: Steps in repair of provisional restorative materials.
Place the fractured pieces of the sample in the mould as fit. Mark a line on each side at a distance of 1mm from the fracture point. Trim the sample at these lines. The edges to be repaired are at 2mm distance from each other. Mark a point along the length of the sample equal to the thickness (2.5mm). Draw a line parallel to the end at this pointJoin the upper end of this line and the lower end of the finished edge to be repaired Trim the angle freeh and to get a 45° bevel.
[Table/Fig-1]: Custom made metal mould. [Table/Fig-2]: Total specimens for polymethyl methacrylate materials and bis-acrylic provisional restorative materials. [Table/Fig-3]: Placement of sample in UTM machine. Journal of Clinical and Diagnostic Research. 2016 Aug, Vol-10(8): ZC72-ZC77
Ankita Singh and Sandeep Garg, Comparative Evaluation of Flexural Strength of Provisional Crown and Bridge Materials- An In-vitro Study Post Hoc Test
Max Stress At 24 Hours
Mean (N/mm )
[Table/Fig-5]: Maximum stress values recorded for various test materials. ANOVA at 24 hours Max stress
Sum of Squares
POST HOC TEST